HAL Id: hal-01157516
Submitted on 28 May 2015
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Cation Intercalation and High Volumetric Capacitance
of Two-Dimensional Titanium Carbide
Maria R. Lukatskaya, Olha Mashtalir, Chang E. Ren, Yohan Dall’Agnese,
Patrick Rozier, Pierre-Louis Taberna, Michael Naguib, Patrice Simon, Michel
W. Barsoum, Yury Gogotsi
To cite this version:
Maria R. Lukatskaya, Olha Mashtalir, Chang E. Ren, Yohan Dall’Agnese, Patrick Rozier, et al..
Cation Intercalation and High Volumetric Capacitance of Two-Dimensional Titanium Carbide.
Sci-ence, American Association for the Advancement of SciSci-ence, 2013, vol. 341 (n° 6153), pp. 1502-1505.
OATAO is an open access repository that collects the work of Toulouse researchers and
makes it freely available over the web where possible.
This is an author-deposited version published in :
Eprints ID : 13896
To link to this article :
To cite this version :
Lukatskaya, Maria R. and Mashtalir, Olha and Ren, Chang E. and
Dall'Agnese, Yohan and Rozier, Patrick and Taberna, Pierre-Louis
and Naguib, Michael and Simon, Patrice and Barsoum, Michel W.
and Gogotsi, Yury Cation Intercalation and High Volumetric
Capacitance of Two-Dimensional Titanium Carbide. (2013) Science
Magazine, vol. 341 (n° 6153). pp. 1502-1505. ISSN 0036-8075
Any correspondance concerning this service should be sent to the repository
Cation Intercalation and High
Volumetric Capacitance of
Two-Dimensional Titanium Carbide
Maria R. Lukatskaya,1,2Olha Mashtalir,1,2* Chang E. Ren,1,2* Yohan Dall’Agnese,1,2,3,4 Patrick Rozier,3Pierre Louis Taberna,3Michael Naguib,1,2Patrice Simon,3,4
Michel W. Barsoum,1Yury Gogotsi1,2†
The intercalation of ions into layered compounds has long been exploited in energy storage devices such as batteries and electrochemical capacitors. However, few host materials are known for ions much larger than lithium. We demonstrate the spontaneous intercalation of cations from aqueous salt solutions between two-dimensional (2D) Ti3C2MXene layers. MXenes combine 2D conductive carbide layers with a hydrophilic, primarily hydroxyl-terminated surface. A variety of cations, including Na+, K+, NH4+, Mg2+, and Al3+, can also be intercalated electrochemically, offering capacitance in excess of 300 farads per cubic centimeter (much higher than that of porous carbons). This study provides a basis for exploring a large family of 2D carbides and carbonitrides in electrochemical energy storage applications using single- and multivalent ions.
With the increased demand for portable and clean energy, electrochemical ca-pacitors have been attracting attention because of their much greater power density and
cyclability relative to Li batteries (1, 2). However, electrical double-layer capacitors (EDLCs), in which the capacity is due to the electrosorption of ions on porous carbon electrodes, have limited energy density (2). Pseudo-capacitors, in which the capacity is due to redox reactions, provide higher energy densities but usually suffer from shorter cyclic lifetimes. RuO2nanosheets have been used in redox capacitors and have shown impressive capacitance and cyclability, but they are quite expensive to produce (2, 3).
Energy density enhancement of capacitors can be achieved by using hybrid devices, which
combine a battery-like redox electrode and a porous carbon electrode (4). Another approach is to use materials in which charge storage is due to intercalation of ions between atomic layers because the capacitances—even at high discharge rates—are high. For example, nanocrystalline Nb2O5 films with storage capacities of ~130 mAh g−1at rates as high as 10 C (charge/discharge in 6 min) for Li+ions in organic electrolytes have been reported. The specific structure of this ma-terial can best be described as a crystalline net-work with two-dimensional (2D) transport paths for ions between atomic layers; thus, even thick electrodes show excellent behavior (5). Another example is Mg-buserite electrodes, which exhibit good Na+ion intercalation capacitances but have poor electrical conductivities (6). Most materials for electrodes that can provide intercalation or sur-face redox capacitances are poor electronic con-ductors [e.g., graphene oxide or TiO2(7)] or are hydrophobic [e.g., graphene (8)].
Recently, we reported on a large family of 2D materials that we labeled“MXenes,” which combine good electrical conductivities with hy-drophilic surfaces. MXenes are 2D materials syn-thesized by the extraction of the“A” layers from the layered carbides or carbonitrides known as MAX phases. The latter have a general formula of Mn+1AXn(n = 1, 2, 3), where M represents a transition metal; A usually represents a III A or IVA element (such as Al, Ga, Si, or Ge); and X represents C and/or N (9). The MXenes Ti3C2 (10), Ti2C, Ta4C3, TiNbC, and (V0.5Cr0.5)3C2(11), have been fabricated by immersing Al-containing MAX powders in HF solution at room or slightly
elevated temperature (12). This synthesis proce-dure leads to the termination of MXene surfaces by primarily O and/or OH groups with some fluorine present. These terminated MXenes are of the form Mn+1XnTx, where T represents sur-face termination (O, OH, and/or F) andx is the number of termination groups. We recently showed that Ti3C2Txcan be readily and spontaneously in-tercalated with organic molecules such as hydra-zine, dimethyl sulfoxide (DMSO), and urea (13). MXenes have shown promise as electrode materials for Li-ion batteries and Li-ion capac-itors (13, 14). For example, when Li+ions in-tercalate into Ti3C2Tx, a steady-state capacity of ~ 410 mAh g−1at 1 C is obtained for additive-free flexible electrodes (13). Furthermore, theoretical calculations have predicted that Li+ions should diffuse rapidly on Ti3C2surfaces, as well as result in high storage capacities (15). However, spon-taneous intercalation of cations from aqueous solu-tions has neither been theoretically predicted nor experimentally demonstrated.
Here, we report on the intercalation of Li+, Na+, Mg2+, K+, NH4+, and Al3+ions between the 2D Ti3C2Txlayers (Fig. 1A). In most cases, the cations intercalated spontaneously. A sche-matic of the process is shown in Fig. 1B. The intercalation of some ions, notably Al3+, can ad-ditionally be promoted electrochemically. We also report on intercalation-induced high capacitances of flexible Ti3C2Txpaper electrodes in aqueous electrolytes.
A large number of salts, bases, and acids were explored (table S1). X-ray diffraction (XRD) pat-terns showed that, after placing the Ti3C2Txin various salt solutions (fig. S1, A to C), there was a downshift in the (0002) peak position. This downshift shows that in all cases, there was an increase in thec-lattice parameter. For exam-ple, thec value of Ti3C2Txincreased from 20.3 Å to as much as 25.4 Å when placed in potassium hydroxide (KOH) and ammonium hydroxide (NH4OH) solutions (fig. S1A). In addition to the compounds listed in fig. S1, A to C, other salts intercalated spontaneously when the MXene powders were immersed in sodium carbonate (Na2CO3), sodium hydroxide (NaOH), or lithium hydroxide (LiOH) solutions.
Not all salts behaved similarly. In the case of high-pH solutions such as KOH, NH4OH, NaOH, LiOH, and several others (table S1), the changes in the interplanar spacing were large (fig. S1A). Conversely, close-to-neutral solutions such as Na,
K, and Mg sulfates resulted in smaller changes inc (fig. S1B; see also table S1). No shift in the (0002) peak positions was observed when Ti3C2Txwas immersed in acetic or sulfuric acid.
To shed light on whether the cations or anions intercalated the Ti3C2Tx layers, we tested three sodium salts with differing anion radii. The re-sults (fig. S1C) showed that thec-axis expansions were comparable and independent of anion radii. Furthermore, energy-dispersive x-ray spectros-copy analysis of Ti3C2Txafter treatment in the different sulfate salts (fig. S1B) confirmed the presence of the cations; sulfur was not detected (table S2), confirming that it is the cations that intercalate between the Ti3C2Txlayers.
Materials with large specific surface area are typically needed to obtain large capacitances in carbon materials for EDLCs. However, at 23 m2/g, the surface area of multilayer exfoliated Ti3C2Tx is low (13). It follows that if double-layer capac-itance were the only operative mechanism, one would expect the capacitance for this material to be less than that of (for example) activated graphene by a factor of 100 (16). However, as noted above, intercalation capacitance can by far exceed double-layer capacitances calculated sole-ly on the basis of a material’s surface area (6, 17). To test this idea, we fabricated multilayer Ti3C2Txelectrodes (see supplementary materials for details) and tested them in NaOH-, KOH-, and LiOH-containing electrolytes using a stan-dard three-electrode asymmetrical setup with an Ag/AgCl reference electrode (fig. S2). The re-sulting cyclic voltammograms (CVs) are shown in Fig. 2A [see fig. S4 for the corresponding electrochemical impedance spectroscopy (EIS) results]. The rectangular-shaped CVs indicate capacitive behavior in these basic solutions. Note that in all experiments, the open circuit potential (OCP) was taken as the starting potential for the CV scans because 0.1 V above this potential, Ti3C2Txoxidation is observed in aqueous electro-lytes (see fig. S3).
To study the effect of a cation’s valence on the electrochemical performance of multilayer exfoliated Ti3C2Txelectrodes, we performed CV scans in 1 M solutions of potassium and aluminum sulfates and nitrates (Fig. 2B and fig. S4B). Clearly, the responses in the K+- and Al3+-containing solutions were distinctively different, confirming once again that the cations (and not the anions) are intercalating. The CV plots for K2SO4are al-most perfectly rectangular. Conversely, the CV
data for the more acidic (see table S3) and less conductive Al2(SO4)3electrolyte yield capac-itance values that are significantly lower, and the shape of the CVat 10 mV/s and the EIS results show a higher resistance (Fig. 2B and fig. S4B). To ensure that lower electrolyte conductivity did not limit the capacitive performance, we tested Ti3C2Txin 1 M Al(NO3)3, which has a conduc-tivity similar to that of 1 M K2SO4(table S3). Although the normalized capacitance did not in-crease appreciably, the CV loops were definitely more rectangular (Fig. 2B), demonstrating the role of electrolyte conductivity.
Further evidence for cation intercalation and its beneficial effect on capacitance comes from the observation that for some electrolytes, time was needed to reach a steady state or maximum capacitance. For strongly basic electrolytes (table S1), such as KOH solutions, the rectangular CV plots were observed almost immediately and the capacitances did not change with time or cycle number. For other electrolytes, however, there was a slow and gradual increase in capacitance with time. For example, for salts such as MgSO4, the CV area increased steadily with time and the maximum capacity was reached only after 48 hours (see figs. S5 and S6). Unlike what is observed for graphite (18), there was no irreversible capac-itance loss during the first cycle for any of the electrolytes studied.
The performance of the multilayer Ti3C2Txin all tested electrolytes is summarized in Fig. 2C. The specific capacitances were calculated by in-tegrating the discharge portions of the CV plots. The results clearly showed responses that de-pended on the electrolytes used. Moreover, the calculated capacitances were quite high for a material with such low surface area.
In situ XRD studies of the intercalation pro-cess during cycling showed that electrochemical cycling leads to insignificant changes in thec values. For example, when a Ti3C2Txelectrode was cycled in a KOH-containing electrolyte, the c values fluctuated within 0.33 Å as the potential was scanned from–1 to –0.2 V (Fig. 3A). Inter-estingly, a slight shrinkage inc values was ob-served with increasing voltage. Similar behavior was observed when Ti3C2Txwas cycled in NaOAc-containing electrolyte (fig. S7). The simplest explanation for this observation is that the pos-itively charged ions incorporated in Ti3C2Tx in-crease the electrostatic attraction between layers, in a manner analogous to what is observed for Fig. 1. Intercalation of
multi-layer exfoliated Ti3C2Tx. (A) Scanning electron micrograph of the Ti3C2Txlayered particle. Inset is a schematic of the same, show-ing the 2D nature of MXenes. (B) Schematic illustration of the intercalation of cations between Ti3C2Tx layers. The interlayer spacing d increases after ion intercalation.
MnO2(19). When Ti3C2Txwas electrochemical-ly cycled in a MgSO4-containing solution, the shift of the (0002) peak almost doubled relative to the KOH and NaOAc electrolytes (compare Fig. 3A and Fig. 3B). Here again, a slight shrink-age in c values was observed with increasing voltage.
To gain further insight into the capacitances and what influences them, we tested MXene “paper” produced by filtering delaminated Ti3C2Tx (Fig. 4B). This paper, with a specific surface area of 98 m2/g, is flexible (inset in Fig. 4B), hy-drophilic, additive-free, and conductive. When tested in KOH, the CVs were rectangular, simi-lar to those obtained when multilayer Ti3C2Tx powder was used (compare Fig. 4C to Fig. 2A). Furthermore, the EIS results indicated that the Ti3C2Txpaper–based capacitors were less resistive (Fig. 4D) than those made with mul-tilayer Ti3C2Tx(fig. S4A). This improved electro-chemical response can be related to a number of factors, such as the absence of a binder in the system, good contact between the restacked flakes in the paper, increased accessibility of the structure, and thinner electrodes (Fig. 4, A and B).
As shown in Fig. 4E, the use of Ti3C2Tx paper electrodes instead of multilayer exfoliated Ti3C2Tx in some electrolytes (e.g., KOH and NaOAc) roughly doubled the gravimetric capac-itance (see fig. S8 for more information about the performance of Ti3C2Tx paper in NaOAc and MgSO4). Even more impressively, the volumet-ric capacitance values recorded for few-layer Ti3C2Txwere on the order of 340 F/cm3for KOH (Fig. 4C and fig. S9). Those values are much higher than those found for activated graphene [60 to 100 F/cm3(15, 20)] or micrometer-thin carbide-derived carbon electrodes [180 F/cm3 (21, 22)]. Extreme values for MnO2hybrid elec-trodes [1200 F/cm3(23); 640 F/cm3(24)] were obtained on thin films of supported nanoparticles, and therefore cannot be compared with our electrodes. A capacitance retention test per-formed by galvanostatic cycling at 1 A/g showed almost no degradation in performance after 10,000 cycles (Fig. 4F).
Our results show that a variety of cations of various charges and sizes can readily intercalate, from aqueous solutions, both multilayer exfoli-ated Ti3C2Tx and MXene paper made of few layers of Ti3C2Tx. The phenomenon depends on pH and the nature of the cations. Extensive in-vestigation of the electrochemical properties of the Ti3C2Txin these aqueous electrolytes showed notable intercalation capacitances. The best per-formance was observed in basic solutions, such as KOH and NaOH for binder-free Ti3C2Tx paper. The latter is highly flexible and yielded volumetric capacitance of up to 350 F/cm3.
As noted, eight MXenes have been reported to date (10) and many more have been theoret-ically predicted (25, 26). Thus, the volumetric capacitances described above are probably far from the maximum values possible for MXenes
in general. The flexibility of Ti3C2Txpaper (Fig. 4B) also opens the door for the use of MXenes in flexible and wearable energy storage devices (27). The fact that a variety of ions, as different as Na+and Al3+, can be accommodated between the MXene layers may also enable MXene use
in batteries as well as in metal-ion capacitors (battery-supercapacitor hybrids). Thus, this work opens up exciting possibilities of developing im-proved intercalation electrodes for batteries, su-percapacitors, and hybrid devices using a large variety of ions and/or electrode chemistries. Fig. 2. Electrochemical performance of Ti3C2Tx
-based supercapacitors in various aqueous elec-trolytes. (A) CV profiles in NaOH-, KOH-, and LiOH-containing solutions at 20 mV/s. (B) CV profiles in K2SO4, Al2(SO4)3, and Al(NO3)3 solu-tions at 20 mV/s. (C) Summary of rate perform-ances in different aqueous electrolytes.
Fig. 3. Electrochemical in situ x-ray diffraction study of multilayer exfoliated Ti3C2Tx. (A) Ti3C2Tx in 1 M KOH solution; (B) Ti3C2Txin 1 M MgSO4solution. Vertical dashed lines indicate the original position of the (0002) peak of the Ti3C2Txelectrodes before mounting in a cell. Inclined arrows show the direction of the (0002) peak shift. Insets illustrate cycling direction and concomitant changes in c lattice parameters during cycling. In both KOH and MgSO4electrolytes, shrinkage during cathodic polarization is observed.
References and Notes
1. B. Conway, Electrochemical Supercapacitors: Scientific Fundamentals and Technological Applications (Kluwer Academic/Plenum, New York, 1999).
2. P. Simon, Y. Gogotsi, Nat. Mater. 7, 845–854 (2008). 3. I. E. Rauda, V. Augustyn, B. Dunn, S. H. Tolbert,
Acc. Chem. Res. 46, 1113–1124 (2013).
4. K. Naoi, W. Naoi, S. Aoyagi, J. I. Miyamoto, T. Kamino, Acc. Chem. Res. 46, 1075–1083 (2013).
5. V. Augustyn et al., Nat. Mater. 12, 518–522 (2013). 6. Z. J. Sun et al., J. Power Sources 216, 425–433 (2012). 7. S. Stankovich et al., Nature 442, 282–286 (2006). 8. D. Li, M. B. Müller, S. Gilje, R. B. Kaner, G. G. Wallace,
Nat. Nanotechnol. 3, 101–105 (2008).
9. M. W. Barsoum, T. El-Raghy, Am. Sci. 89, 334 (2001). 10. M. Naguib et al., Adv. Mater. 23, 4248–4253 (2011). 11. M. Naguib et al., ACS Nano 6, 1322–1331 (2012). 12. O. Mashtalir, M. Naguib, B. Dyatkin, Y. Gogotsi,
M. W. Barsoum, Mater. Chem. Phys. 139, 147–152 (2013).
13. O. Mashtalir et al., Nature Commun. 4, 1716 (2013). 14. J. Come et al., J. Electrochem. Soc. 159, A1368–A1373
15. Q. Tang, Z. Zhou, P. W. Shen, J. Am. Chem. Soc. 134, 16909–16916 (2012).
16. Y. Zhu et al., Science 332, 1537–1541 (2011). 17. L. Mai et al., Sci. Rep. 3, 1718 (2013). 18. P. W. Ruch et al., Carbon 48, 1880–1888 (2010). 19. O. Ghodbane, F. Ataherian, N.-L. Wu, F. Favier, J. Power
Sources 206, 454–462 (2012).
20. S. Murali et al., Nano Energy 10.1016/j.nanoen. 2013.01.007 (2013).
21. J. Chmiola, C. Largeot, P.-L. Taberna, P. Simon, Y. Gogotsi, Science 328, 480–483 (2010).
22. M. Heon et al., Energy Environ. Sci. 4, 135 (2011). 23. X. Lang, A. Hirata, T. Fujita, M. Chen, Nat. Nanotechnol.
6, 232–236 (2011).
24. X. Zhao et al., ACS Nano 6, 5404–5412 (2012). 25. M. Kurtoglu, M. Naguib, Y. Gogotsi, M. W. Barsoum,
MRS Commun. 2, 133–137 (2012).
26. M. Khazaei et al., Adv. Funct. Mater. 23, 2185–2192 (2012).
27. J. R. Miller, Science 335, 1312–1313 (2012). Acknowledgments: We thank B. Duployer and J. Come at Paul Sabatier University for help in electrochemical experiments, V. N. Mochalin and M. Beidaghi for helpful discussions, and the Centralized Research Facility of Drexel
University for access to XRD and SEM equipment. MXene synthesis was funded by the U.S. Department of Energy, Office of Vehicle Technologies, Batteries for Advanced Transportation Technologies (BATT) Program, under contract DE-AC02-05CH11231, subcontract 6951370. M.R.L. was supported by the U.S. Department of Energy, Energy Storage Systems Research Program, through Sandia National Laboratory. P.S. was supported by the European Research Council (advanced grant ERC-2011-AdG, project 291543–IONACES) and the Chair of Excellence “Embedded multi-functional nanomaterials” from the EADS Foundation. Collaboration between Drexel University and Paul Sabatier
University was supported by the Partner University Fund of the Embassy of France.
www.sciencemag.org/content/341/6153/1502/suppl/DC1 Materials and Methods
Supplementary Text Figs. S1 to S9 Tables S1 to S4 References (28, 29) 10.1126/science.1241488 st Fig. 4. Electrochemical performance
of binder-free Ti3C2Txpaper elec-trodes: (A) Schematic of electrode fabrication. During the first stage, the multilayer Ti3C2Tx powders are delam-inated to produce few-layer MXene flakes (see supplementary materials); the result-ing colloidal solution is filtered through a porous membrane, producing binder-and additive-free Ti3C2Txpaper elec-trodes for further use in capacitance tests. (B) Scanning electron micrograph of paper electrode. Inset is a photograph of the paper showing its flexibility. (C) CV of Ti3C2Txpaper in KOH electrolyte. (D) EIS data in KOH for Ti3C2Txelectrode (KOH, solid symbols) and Ti3C2Txpaper (p-KOH). (E) Rate performance of the Ti3C2Txpaper (open symbols) versus mul-tilayer exfoliated Ti3C2Txelectrode (solid symbols) in KOH-, MgSO4-, and NaOAc-containing electrolytes. (F) Capacitance retention test of Ti3C2Txpaper in KOH. Inset: Galvanostatic cycling data collected at 1 A/g.